Author
tranxuyen
View
221
Download
2
Embed Size (px)
Int J Fract (2010) 162:229244DOI 10.1007/s10704-010-9442-4
ORIGINAL PAPER
Studies of dynamic crack propagation and crack branchingwith peridynamics
Youn Doh Ha Florin Bobaru
Received: 31 August 2009 / Accepted: 5 January 2010 / Published online: 20 January 2010 Springer Science+Business Media B.V. 2010
Abstract In this paper we discuss the peridynamicanalysis of dynamic crack branching in brittle materialsand show results of convergence studies under uniformgrid refinement (m-convergence) and under decreas-ing the peridynamic horizon (-convergence). Com-parisons with experimentally obtained values are madefor the crack-tip propagation speed with three differentperidynamic horizons. We also analyze the influence ofthe particular shape of the micro-modulus function andof different materials (Duran 50 glass and soda-limeglass) on the crack propagation behavior. We show thatthe peridynamic solution for this problem captures allthe main features, observed experimentally, of dynamiccrack propagation and branching, as well as it obtainscrack propagation speeds that compare well, quali-tatively and quantitatively, with experimental resultspublished in the literature. The branching patterns alsocorrelate remarkably well with tests published in theliterature that show several branching levels at higherstress levels reached when the initial notch starts prop-agating. We notice the strong influence reflecting stresswaves from the boundaries have on the shape andstructure of the crack paths in dynamic fracture. Allthese computational solutions are obtained by usingthe minimum amount of input information: density,elastic stiffness, and constant fracture energy. No spe-cial criteria for crack propagation, crack curving, or
Y. D. Ha F. Bobaru (B)Department of Engineering Mechanics, Universityof NebraskaLincoln, Lincoln, NE 68588-0526, USAe-mail: [email protected]
crack branching are used: dynamic crack propagationis obtained here as part of the solution. We concludethat peridynamics is a reliable formulation for model-ing dynamic crack propagation.
Keywords Dynamic fracture Crack branching Brittle fracture Peridynamics Nonlocal methods Meshfree methods
1 Introduction
1.1 Literature review of dynamic crack propagation
In a brittle material, a propagating crack can departfrom its original straight trajectory and curve or splitinto two or more branches. Under very high states ofstress, the propagating crack will divide into a river-delta crack pattern (Bowden et al. 1967; Ramulu andKobayashi 1985). This fragmentation of highly loaded,brittle materials is often a succession of multiplebranching of what was initially a single crack. Increasesin the roughness of the fracture surface prior to branch-ing were consistently observed in all reported inves-tigations (Ramulu and Kobayashi 1985; Dll 1975).In crack branching of edge notch specimens of brit-tle materials it has also been observed that the crack tipvelocity drops by no more than 510% in the branchingregion (Dll 1975).
In atomistic models, under conditions that lead toinstability of the crack path, cracks can branch without
123
230 Y. D. Ha, F. Bobaru
a specific criterion (see Zhou et al. 1996). Particle-typemodels (see Bolander and Saito 1998) are also capa-ble of simulating crack branching. However, none ofthese methods is able to capture the crack propaga-tion speed or the angle of crack branching correctly.For instance, MD simulations show instabilities thatlead, shortly after the bifurcation of a crack, to thepropagation of only one of the two branches, the otherbeing arrested. Moreover, the branching angle com-puted with MD (see Zhou et al. 1996) is greater than90, whereas experiments show much smaller crackbranching angles (Ramulu and Kobayashi 1985). Onemay ask whether quantum mechanical calculations areneeded to predict the phenomenon of dynamic frac-ture in brittle materials (see Cox et al. 2005) whichis one of the great challenges in dynamic fracture.One likely reason for MD simulations failure to cor-rectly predict dynamic fracture is that, for example,crack branching events are controlled by the interac-tion and wave reflections from the boundaries (Ravi-Chandar 1998). Because of this, one would have toeither model the entire structure with MD (not a via-ble option) or use a multiscale model that is capableof transferring the waves between the scales correctly(still an open problem). Numerical simulations basedon continuum methods of dynamic crack propagationbehavior have been very difficult to develop and, tothis date, a reliable method for simulating this complexproblem has not been found in spite of considerableefforts in this direction (e.g. Xu and Needleman 1994;Camacho and Ortiz 1996; Ortiz and Pandolfi 1999;Belytschko et al. 2003; Rabczuk and Belytschko 2004;Song et al. 2006). All these methods use some versionof cohesive-zone models. As such, they all modify thelocal continuum mechanics equations and introduce anonlocal effect given by the parameters and length-scales in the cohesive-zone model. To reduce meshdependency when the grids are refined special meth-odologies have to be used (Zhou and Molinari 2004).For the existing approaches, the difficulties in mod-eling dynamic fracture processes like crack branch-ing are many. For example, continuum-type methodsusing the cohesive FEM or the XFEM require a dam-age criterion and a tracking of the stresses around thecrack tip to decide when to branch the crack. Decisionsalso have to be taken in terms of the angle of propa-gation of the branches and about how many brancheswill be allowed to form. In methods in which the crackadvances along the element sides by separating
elements from one another, the crack path becomesnon-smooth (see Xu and Needleman 1994; Camachoand Ortiz 1996; Ortiz and Pandolfi 1999). Since thecorrect path (which minimizes the strain energy) ofthe crack propagation is not computed correctly, thereare significant departures from the true energy releasedduring the crack propagation event. In such cases, reli-able prediction of strength of brittle ceramics underimpact, for example, becomes difficult. Mesh depen-dency is an additional problem in cohesive-zone FEM-based methods. Important progress has been recentlymade by using the XFEM method which allows cracksto pass through the finite elements (see e.g. Belytschkoet al. 2003). Subdivision of the cut elements for numer-ical integration purposes increases the complexity andthe cost of the method. This method requires phenom-enological damage models and branching criteria, aswell as tracking of the crack path using level sets, forexample. It is not yet clear if the method is applicableto problems that involve fragmentation and/or multi-ple crack interactions, branching, and coalescence. Themethod does not predict the experimentally observedcrack propagation speeds (see Song et al. 2008). Cohe-sive-zone based models need to modify the experi-mental values of the fracture energy by several factorsin order to get propagation velocities in the range ofmeasured ones (Song et al. 2008).
In the present contribution we try to answer whetherquantum, atomistic, or multiscale models are neededin dynamic fracture in order to correctly simulate theobserved crack propagation velocities and crack paths(Cox et al. 2005; Song et al. 2008). We will show thatperidynamics is able to correctly model and simulatedynamic fracture, in particular crack branching in brit-tle materials. Peridynamics, which is a reformulationof continuum mechanics (Silling 2000; Silling et al.2007b), does not require criteria for crack propagationor crack branching: these happen spontaneously in thismethod and are autonomously generated by a simplebond-failure criterion that is correlated to the materialsenergy release rate. The name peridynamics comesfrom the Greek peri which means nearby, anddynamics. Peridynamics is a nonlocal method in whichmaterial points interact not only with their nearestneighbors but also with points nearby, inside a horizon.This is what physically happens at the atomic scale, forexample, but peridynamics extends this idea to the con-tinuum scale. We will show convergence in terms of thecrack path and the crack propagation speed under grid
123
Studies of dynamic crack propagation 231
refinement (the so-called m-convergence, Bobaru et al.2009) and under decreasing peridynamic horizon (theso-called -convergence, Bobaru et al. 2009). The crackbranching patterns obtained using peridynamics followremarkably close the experimental results which showsecondary branching taking place when higher stresslevels are reached at the tip of the pre-notch prior tocrack propagation. Moreover, the only input parame-ters in the model are the Youngs modulus, the density,and the fracture energy (which is kept constant, and nota function of the propagation velocity or of the incurreddamage, in this first study).
The paper is organized as follows: in the next sec-tion we describe the sample problem setup. In Sect. 2we briefly review the peridynamic formulation and theconnections between the parameters in the formula-tion and the material properties like the energy releaserate. In Sect. 3 we present the numerical results for theconvergence studies. We look at both the crack pathand the propagation speed of the crack, as measures ofconvergence. In Sect. 4 we analyze the influence of themicro-modulus function on crack branching results aswell as the solutions for two different brittle materialsunder higher loading conditions that lead to cascadingbranching. We also comment on the roughening zonesthat take place in the branching regions and on the effectof the reflection waves on the propagation paths of thedynamic cracks. The conclusions are given in Sect. 5.
1.2 Problem setup
We consider the following setup as a benchmark prob-lem for analyzing crack branching phenomena: a pre-notched thin rectangular plate with 0.1 m by 0.04 m asshown in Fig. 1. All simulations in this paper are 2Dsimulations. For some 3D results we refer the read-ers to Ha et al. (2010). The materials chosen for thisstudy are selected because for these materials there areexperimental results published on the crack propaga-tion velocity in the region of branching or the maximumpropagation velocity measured. The two materials usedhere are a Duran 50 glass (taken form Dll 1975) and asoda-lime glass (taken from Bowden et al. 1967). Thematerial properties are summarized in Table 1. Pleasenote that in the bond-based peridynamic implementa-tion used here, the numerical models will be limited tousing a fixed Poisson ratio of 1/3 (for 2D plane stressproblems). If other Poisson ratios are desired, then the
Fig. 1 Description of the problem setup for the crack branchingstudy
state-based peridynamics formulation should be used(see Silling et al. 2007b). For dynamic fracture prob-lems, the Poisson ratio value does not have a significantinfluence on the propagation speed or the crack pathshapes (Silling et al. 2007a).
In the experimental settings the loading of the sam-ple may take tens of seconds or more. In explicitdynamic simulations that would be too expensive tocompute. Instead, we choose to apply, along the upperand lower edges (see Fig. 1), traction loadings sud-denly at the initial time step and maintain this load-ing constant after that. The theoretical background forthe peridynamics analysis is based on Sillings origi-nal peridynamics paper (Silling 2000), the impositionof the traction boundary conditions is as in Ha andBobaru (2009), and the numerical implementation offailure is like in Silling and Askari (2005). The samegeometrical setup for studying crack branching simu-lations has been used in other studies (Belytschko etal. 2003; Rabczuk and Belytschko 2004; Song et al.2006).
While there is no analytical solution for the crackbranching problem, we can compare our simulationresults with experiments. Unfortunately, the experi-mental papers we found do not provide a completedescription of the conducted experiment on crackbranching: some papers show the crack paths but donot provide crack propagation speed data, others givethe propagation speed but do not show the crack paths,and most do not describe in detail the loading condi-tions. We decided to perform the peridynamic simula-tions using a setup similar to that used in a few recentsimulation papers (Belytschko et al. 2003; Rabczukand Belytschko 2004; Song et al. 2006). The materialparameters, however, are like those used in the exper-iments (Bowden et al. 1967; Dll 1975). The maxi-mum crack propagation speed, or the crack propagation
123
232 Y. D. Ha, F. Bobaru
Table 1 Material properties for Duran 50 and soda-lime glasses
Density () (kg/m3) Youngs modulus (E) (GPa) Poisson ratio () Fracture energy (G0) (J/m2)
Duran 50 glass 2,235 65 0.2 204
Soda-lime glass 2,440 72 0.22 135
speed in the region of branching, is data that is fairlyreproducible in experiments and this is reported inBowden et al. (1967) and Dll (1975), for example.We are not aware of any numerical method that canreproduce the experimentally measured dynamic crackpropagation velocity. Note that in previous studies, forcertain methods, the fracture energy has to be signif-icantly modified (by several factors) in order to bringthe dynamic crack propagation speed closer to the mea-sured values (see, e.g. Belytschko et al. 2003; Rabczukand Belytschko 2004).
2 The peridynamic formulation
The peridynamic formulation (Silling 2000) relies onintegration of forces acting on a material point and thusit does not face any of the mathematical inconsistenciesseen in the classical continuum mechanics equations.The integration takes place over a horizon (which,in principle, extends to infinity but, for convenienceis finite) within which the material points are inter-acting with each other. In certain problems, the sizeof the horizon can be correlated to an intrinsic materiallength-scale. However, in many cases a material length-scale is not visible either because the micro-structureand the specific loading and boundary conditions donot lead to a measurable effect of the length-scale. Insuch cases, the horizon is selected by the user accord-ing to convenience (see Bobaru et al. 2009). Allowing avariable horizon (with a correspondingly scaled micro-modulus parameter) defines a way of introducing adap-tive refinement for this nonlocal method. It is importantto notice that peridynamics is a continuum theory, nota particle-type method. This allows the convergenceresults of the peridynamic solution to the classical elas-ticity solutions in the limit of the horizon going to zero(Bobaru et al. 2009; Silling and Lehoucq 2008).
An important advantage of peridynamics is the waydamage is introduced: material points are connectedwithin the horizon via elastic (linear or nonlinear)bonds that have a critical relative elongation, s0, at
which they break (Silling 2000). The critical relativeelongation for brittle materials is computed from theexperimentally measured value of the fracture energyfor a specific material (Silling and Askari 2005). Dam-age is implemented as the fraction between the numberof broken bonds and the number of initial bonds (Sillingand Askari 2005). Cracks in peridynamics form as sur-faces between material points form, as a consequenceof sequential breaking of bonds. Thus, there is no needto track the cracks like in other continuum methods,or to impose criteria for when cracks should branch,change direction, turn, coalesce, etc. Moreover, peri-dynamics allows for spontaneous generation of crackswhere no flaws were present before. This is shown, forexample, in Silling et al. (2009) for the crack nucleationand in simulation of spallation (see Xie 2005) wherespallation is treated as real fracture and not modeledby void-growth formulations as in existing literatureresults.
We now briefly review the peridynamic formulationbased on Sillings original peridynamics paper (Silling2000). Also, we consider the summary of the numeri-cal implementation of the traction boundary conditionsin peridynamics (Ha and Bobaru 2009) and the formu-lation for the damage model in peridynamics (Sillingand Askari 2005).
The peridynamic equations of motion are given by:
u (x, t) =
Hf(u
(x, t
) u (x, t) , x x)dx
+b (x, t) (1)where f is the pairwise force function in the peridy-namic bond that connects node x to x and u is the dis-placement vector field. is the density and b (x, t) isthe body force. The integral is defined over a region Hcalled the horizon, which is the compact supporteddomain of the pairwise force function around point x.
A micro-elastic material (Silling 2000) is defined asone for which the pairwise force derives from a poten-tial :
f (, ) = (, )
(2)
123
Studies of dynamic crack propagation 233
where = xx is the relative position in the referenceconfiguration and = u u is the relative displace-ment. A linear micro-elastic potential is obtained if wetake
(, ) = c () s2
2(3)
where = and the relative elongation of a bond is
s =
(4)
where = + . The function c () is calledmicro-modulus and has the meaning of the bond elasticstiffness. There are various formulations for the micro-modulus function and in Sect. 4.1 we perform tests fordynamic crack propagation to assess the influence ofthe particular shape of the micro-modulus function onthe crack path structure. We will observe that the crackpropagation speed is not influenced by the shape of themicro-modulus, once the horizon is reasonably smallcompared to the dimensions of the structure analyzed.The pairwise force corresponding to a linear micro-elastic potential has the following form:
f (, ) ={
++c () s, 0, >
(5)
where is the radius of the horizon region (which wewill also refer to as the horizon). In this paper, we usethe constant and conical 2D micro-modulus functions(see Fig. 2). Following the same procedure performedto calculate the micro-modulus function in 1D (Bobaruet al. 2009), we obtain the constant micro-modulusfunction in 2D, plane stress conditions:
c () = c0 = 6E3 (1 ) (6)
Similarly, the conical micro-modulus function isobtained as
c () = c1(
1
)= 24E
3 (1 )(
1
)(7)
The shapes of the constant and conical micro-mod-ulus functions are illustrated in Fig. 2.
In the bond-based peridynamics, any particle insidethe horizon of another particle interacts only through acentral potential. This assumption results (for an isotro-pic, linear, micro-elastic material) in an effective Pois-son ratio of 1/3 in 2D (and 1/4 in 3D), but this limitationis readily eliminated by using the state-based peridy-namics (Silling et al. 2007a,b). In this paper, we utilize
Fig. 2 Constant (left) and conical (right) micro-modulus func-tions
the bond-based peridynamics, thus, in all the reportedsimulations here the effective Poisson ratio is 1/3.
In order to introduce failure into the peridynamicmodel, we consider that the peridynamic bonds canbe broken when they are stretched beyond a predefinedlimit. We call this limit the critical relative elongation,s0. According to Silling and Askari (2005), there is noforce sustained by the bond after its failure. Also, oncea bond fails, it is failed forever; this makes the modelhistory dependent. To completely separate a body intotwo halves across a fracture plane requires breaking allthe bonds that initially connected points in the oppositehalves (see Silling and Askari 2005). The energy perunit fracture length (in 2D, fracture area in 3D) for com-plete separation of the two halves of the body is calledfracture energy, G0. In 3D, Silling and Askari relatethe critical elongation, s0, with this measurable quan-tity (G0) (Silling and Askari 2005). In 2D with planestress conditions, the fracture energy can be derived as
G0 = 2
0
z
cos1
(z
)
0
[c () s20
2
]dddz (8)
(See Fig. 3 for an explanation of this computa-tion.) Substituting the constant micro-modulus func-tion (Eq. 6) and rearranging for s0, we can rewrite thisequation to obtain s0
s0 =
4G09E
(9)
In similar way, the critical relative elongation for theconical micro-modulus function (Eq. 7) is
s0 =
5G09E
(10)
The critical relative elongation depends on the mate-rial properties and the horizon . Note that as the hori-zon goes to zero, the critical relative elongation goes toinfinity, thus breaking such bonds requires larger and
123
234 Y. D. Ha, F. Bobaru
Fig. 3 Evaluation of fracture energy. For each point A along thedashed line, 0 z , the work required to break the bondsconnecting A to each point B in the circular cap is given by Eq. (8)
larger forces. This agrees with the physical experienceat atomic and subatomic scales where, in order to breakapart smaller and smaller sized bonds, one needs higherand higher forces. The values for the fracture energyused in this paper are the ones given in Dll (1975)for Duran 50 glass and soda-lime glass materials andmeasured at the instant of crack branching of a dynami-cally running crack. Note that there is evidence that thefracture energy varies with the crack propagation speed(see, e.g. Dll 1975). However, other authors point outthe fact that the apparent increase in the fracture energywith crack speed may be due to the presence of micro-cracks (see, e.g. Cox et al. 2005; Ravi-Chandar 1998).For simplicity, in this work, we keep the fracture energyconstant and equal to that measured at crack branching.Nevertheless, it is very easy to introduce the velocity-dependent fracture energy (Dll 1975) in our modeland we plan to do so in the future. Moreover, it hasbeen observed that peridynamics generates fragmentsize distributions closer to experimentally measuredones if the critical relative elongation (and therefore thefracture energy) depends on the damage index (ratio ofnumber of broken bonds and number of initial intactbonds) in the following way: if the damage index islarger than some fraction (say 0.2) then the critical rel-ative elongation value increases with the damage index(see Silling 2005). Such damage-dependent model isused in Ha and Bobaru (2010) for dynamic fractureproblems. Note that other models have been used inthe past to explain dynamic instabilities (see Buehleret al. 2003) in dynamic crack propagation using MDmodels, but this does not appear to be needed in peri-dynamics to trigger instabilities or crack branching.
Additionally, since we apply the load abruptly alongthe upper and bottom boundaries, relatively high tensilestress act along these boundaries (see the first figure (a)
in Fig. 4) at the early stages of the simulation. In orderto prevent tearing of the first few layers of nodes fromthe rest of the plate we set the boundary nodes as no-fail zones. In a no-fail zone the damage index is alwayszero. The traction boundary conditions are applied toa single layer of nodes at the surface in peridynamics,which is similar to how one imposes these conditions inthe FEM, for example. The numerical implementationof traction boundary conditions and the convergencestudies are shown in Ha and Bobaru (2009). These loadsare applied suddenly and a shock wave propagates. InFig. 4, we show a few snapshots of the strain energy andclose-ups around the tip of the pre-notch of the damagefor dynamic crack propagation in the setup shown inFig. 1, for Duran glass. The model has a uniform gridspacing with x = 0.125 mm, the horizon = 0.5 mm,and a uniform tensile stress = 12 MPa is applied. InFig. 4a, the colors denote the magnitude of the elas-tic strain energy. In Fig. 4a note the ripples behind thewave-front caused by the wave dispersion which, inperidynamics, is due to the size of the horizon and thesize of the discretization (see discussion of the 1D casein Xie 2005, pp. 4044). The colors in the right-handside plots of Fig. 4 represent damage levels. Right afterthe shock wave reaches the center line, the crack startspropagating (compare Fig. 4a, c at 6 and 9s).
3 Numerical studies of convergence in dynamiccrack branching
In peridynamics, we can talk about three types of con-vergence (see Bobaru et al. 2009 and Fig. 5):
The -convergence: 0 and m(= /x) is fixedor increases with decreasing but at a slower rate.In this case the numerical peridynamic approxima-tion converges to an approximation of the classi-cal solution (if this exists), almost everywhere. Thelarger m is, the closer this approximation becomes.(The convergence is not guaranteed to be uniformin problems with singularities.)
The m-convergence: is fixed and m . Thenumerical peridynamic approximation convergesto the exact nonlocal peridynamic solution for thegiven .
The (m)-convergence: 0 and m increaseswith decreasing , with m increasing faster than decreases. In this case numerical peridynamic
123
Studies of dynamic crack propagation 235
Fig. 4 Elastic strain energyand damage map around thepre-crack tip, at the initialstages of crack propagation( = 0.0005 m,x =0.000125 m, applied load = 12 MPa). a Elasticstrain energy; b Time;c Crack-tip near-view
Fig. 5 Graphicaldescriptions for thea m-convergence andb -convergence
approximation converges to the analytical peridy-namic solution and converges uniformly to the localclassical solution (if this exists), almost everywhere.
Here we are studying the m-convergence and wemake some observations related to the -convergencefor dynamic crack propagation problems. The prob-lem to be analyzed is shown in Fig. 1: an edge-notchplate. One way to introduce a pre-crack in peridynamicmodel is to break all bonds that cross the pre-crack line.Another way is to erase nodes that are along the pre-crack line in addition to breaking all bonds crossing thelines. The first option, under m-convergence, will resultin the same effective pre-crack. The second option,under m-convergence, can also maintain the pre-crackbut only if the total volume of the nodes removedremains the same for any grid spacing used. Note, how-ever, that under -convergence things are more delicate.The reason is that if we change the horizon the damagearea along the pre-crack and in front of the pre-crack tip
changes independent of the way in which we introducethe pre-crack in the peridynamic model.
In Fig. 6, the initial damage areas of two models withdifferent grid spacings are compared. The color-barrepresents damage levels. The thick black line denotesthe pre-notch. The triangles and the squares are nodesof the coarse and fine models, respectively. In Fig. 6a,the damage area of the coarse model matches with thearea of the fine model for the same horizon size of = 2 mm. However, the damage area of the fine modelwith = 1 mm is slightly smaller than the area of thecoarse model with = 2 mm, as shown in Fig. 6b.
3.1 The m-convergence study
For time integration we use an explicit method, theVelocityVerlet algorithm. The VelocityVerlet algo-rithm (Hairer et al. 2003) is:
123
236 Y. D. Ha, F. Bobaru
Fig. 6 Relations between the horizon, grid spacing, and the dam-age area. (triangles nodes of the coarse model, squares nodes ofthe fine model). a Damage areas on two grids with same horizon
( = 0.002 m for both models); b Damage areas on two gridswith different horizons ( = 0.002 m for coarse model, 0.001 mfor fine model)
un+ 12 = un +t
2un (11a)
un+1 = un + t un+ 12 (11b)
un+1 = un+ 12 +t
2un+1 (11c)
where u, u, and u denote the displacement, velocity,and acceleration vectors, respectively.
We perform the m-convergence tests for two differ-ent horizon sizes: = 3 mm and = 2 mm. Please notethat these horizon sizes are relatively large compared tothe structural dimensions. All models have the uniformgrid spacing. A uniform time step size of 25 ns is usedand this is a stable time step for the finest model amongall tests performed in this paper, with = 0.5 mm andm = 4. A uniform tensile stress = 12 MPa is applied(as described in the previous section) for all the testsin this section. All computations in this section use theconstant micro-modulus function (Eq. 6) and the Duran50 glass material parameters.
We first perform the m-convergence study for thefixed horizon = 3 mm. The peridynamic models usedfor this study are the ones with x = 1 mm (4,326nodes), x = 0.5 mm (16,646 nodes), and x =0.25 mm (65,448 nodes). For this test, the model withx = 1 mm has maximum 29 nodes in the horizon(m = 3), the model with x = 0.5 mm has a maximumof 113 nodes in the horizon (m = 6), and the one withx = 0.25 mm has maximum 441 nodes in the horizon(m = 12). The crack paths for these cases at 46 s arecompared in Fig. 7. In all damage map plots we use thesame range for the color-bar of the damage index as inFig. 6. The results in Fig. 7 show that m-convergence
of the crack path is obtained even for m-values as smallas 3. In all cases in Fig. 7, the crack starts propagat-ing around 7 s, and the crack branches around 25 snearby 0.071 m measured from the left-side of the plate.
In these results we notice that a thicker damage zoneis produced before the crack branches. This may be anindication of the fracture surface roughness prior tobranching that is observed consistently in all reportedexperimental investigations of crack branching in brit-tle materials (see, e.g. Ramulu and Kobayashi 1985 andreferences therein).
For the fixed horizon = 2 mm, the m-convergencestudy is performed using the same three numerical gridsas above. Since the horizon is smaller, the correspond-ing m values will be smaller than previously: the coars-est model with x = 1 mm has maximum 13 nodes inthe horizon (m = 2), the one with x = 0.5 mm hasmaximum 49 nodes in the horizon (m = 4), and the onewith x = 0.25 mm has maximum 197 nodes in thehorizon (m = 8). The crack branching path at 40 s forour peridynamic simulations are shown in Fig. 8. Thecrack path given by the coarsest model with m = 2is slightly different from the others, but the paths withm = 4 and 8 are very similar to each other. In Fig. 8,crack branching takes place around 24 s and around0.068 m from the left edge.
These peridynamic results for two different horizonsizes indicate that m-convergence takes place for thedynamic crack branching problem in terms of the crackpath and the crack propagation speed, the latter becausethe crack tip locations at the same times are similaramong the different solutions. This is expected to hold
123
Studies of dynamic crack propagation 237
Fig. 7 Crack pathcomputed with differentgrids for = 0.003 m at46 s. a m = 3, x =0.001 m; b m = 6, x =0.0005 m; c m = 12, x =0.00025 m
Fig. 8 Crack pathcomputed with differentgrids for = 0.002 m at46 s. a m = 2, x =0.001 m; b m = 4, x =0.0005 m; c m = 8, x =0.00025 m
for any given . It appears that m = 4 is a good choicebecause the number of nodes inside horizon allows asufficiently large number of directions along which thetrue crack path can develop. Using a larger value ofm requires higher computational cost, while the resultsare not affected. In all remaining tests we will use thisvalue of m.
3.2 Crack path under changing horizon
The -convergence has to be treated carefully for prob-lems with initial cracks or notches due to the changingsize of the initial damage area as discussed in the begin-ning of Sect. 3 and Fig. 6. The tests in this section arealso for the Duran 50 glass material and the constantmicro-modulus function (Eq. 6).
For a fixed m = 4, the impact of a changing isinvestigated by using the four different kinds of hori-
zons, and therefore, four different grids: the coarsestmodel has = 4 mm with the uniform grid spacingof x = 1 mm (4,326 nodes), the subsequent mod-els have half the horizon size of the previous modeland half the grid spacing. Thus, the other three modelshave, respectively, = 2 mm and x = 0.5 mm (16,646nodes), = 1 mm and x = 0.25 mm (65,448 nodes),and = 0.5 mm and x = 0.125 mm (258,566 nodes).A uniform time step size of 25 ns (which is a stabletime step for the finest model) and the uniform ten-sile stress = 12 MPa are applied for all peridynamicmodels. In all models, the maximum number of nodesin each horizon is 49. The critical relative elongations0 also changes with a decreasing horizon, see Eq. (9).Also, the damage area becomes smaller as the horizondeceases, and this is especially important for the areain front of the pre-crack tip. The -convergence, here,has to be understood within this context. Note that thereexists the possibility that the dynamic fracture behavior
123
238 Y. D. Ha, F. Bobaru
is connected to one or multiple length scales (see, e.g.Livne et al. 2007). Material microstructure is likely toinfluence the dynamic fracture behavior and determineone such physical length scale. The numericalmodels used in the present paper are for an idealhomogeneous material and the crack propagation isgenerated by stress waves interaction due to the shockloading. Notice that crack branching can take placewithout the influence of the stress wave interaction(see Ravi-Chandar and Knauss 1984a). In the futurewe also plan to run simulations with quasi-staticallyapplied loads. The results below indicate that, for suchhomogeneous materials we have -convergence in thedynamic crack branching problem. The question ofwhich material length-scale controls dynamic frac-ture? is left for the future since the picture is com-plicated by how energy is supplied to the region ofthe crack tip (Ravi-Chandar and Knauss 1984b; Ravi-Chandar 1998). In experiments (e.g. Bowden et al.1967) it is delivered via quasi-static loading, while inthe computations here it is delivered by the stress wavesinduced through the shock loading.
The crack path at 46 s for peridynamic simulationsusing four uniform grids are shown in Fig. 9. Noticethat there is a slightly asymmetric path obtained forthe case shown in Fig. 9c. This is due to the coordi-nate system used, the (0, 0) being at the left bottomcorner. When the origin of the coordinate system ismoved to the center of the plate, then the symmetryof the solution is recovered. For all horizons the shapeof the crack path looks almost identical to one another(see the results in Fig. 9). We notice, from monitoringstrain energy plots, that the direction of the crack pathsafter branching is strongly influenced by the reflectionelastic waves from the boundaries. Experimental evi-dence of the influence of the stress wave on the crackpath shape is presented in Ravi-Chandar and Knauss(1984b). The effect is that the branching angle of theinitial cusp-like shape increases as the branches propa-gate. We will see that this effect of the elastic waves onthe crack path propagation after branching is differentfor the soda-lime glass material. The reason is that elas-tic waves propagate faster (due to higher stiffness) andcracks propagate slower in the soda-lime glass com-pared to the Duran glass.
We look now in more detail at the branching events inthe finest model in Fig. 9d. Determining where branch-ing occurs can be done in several ways. One way is toconsider the time when the right-most nodes with
non-zero damage are no longer along the middle line(the direction of the initial crack) but become distrib-uted symmetrically about the mid-line, or the crackdirection just before branching. In Fig. 10, we showthe details of the branching event for the finest model.The branching moment appears to take place between22.5 and 23 s.
3.3 Comparison of peridynamic crack propagationspeed with experimental values
In this section we compare the crack propagation speedfrom the peridynamic simulations with those from theexperiments in Bowden et al. (1967). We examine thesoda-lime glass material with three peridynamic mod-els: a small horizon model with = 0.5 mm (258,566nodes), a medium horizon model with = 1 mm (65,448nodes), and a large horizon model with = 2 mm(16,646 nodes). A uniform tensile stress = 14 MPais applied suddenly along the long sides of the plate(see Fig. 1). The VelocityVerlet method is used witha uniform time step size of 25 ns. The constant micro-modulus function is used.
The crack paths are very similar for all three modelsas shown in Fig. 11ac. We compare the crack propaga-tion speeds in Fig. 11d. Each point on the crack prop-agation speed profiles (blue triangles, green squares,and orange circles in Fig. 11d) is computed by esti-mating the location of the crack-tip (after branchingwe only follow the upper branch) at the time when thedata-dumps are performed. The data-dumps are doneevery 2 s (or every 80 time-steps) starting from theinitial time-step. This implicitly introduces a differencecompared to the actual instantaneous crack propagationspeed. The crack-tip is determined to be the right-mostnode which has the damage index larger than 0.35. Inthe other words, peridynamic bonds related to this nodeare broken over 35% compared to the initial, undam-aged state of the node. The crack propagation speed attl is computed by
V = x x1t t1 (12)
where x and x1 denote the crack-tip positions at thecurrent time t and at the previous data-dump time t1.Here, = 1, . . . , 81 corresponding to the total simu-lation time of 40 s. The dotted line shows the maxi-mum fracture speed 1580 m/s for the soda-lime glassmeasured in experiments (Bowden et al. 1967) where
123
Studies of dynamic crack propagation 239
Fig. 9 Crack branchingpath with various (m = 4)using peridynamic analysisat 46 s. a = 0.004 m, x= 0.001 m; b = 0.002 m,x = 0.0005 m; c = 0.001 m, x =0.00025 m; d = 0.0005 m,x = 0.000125 m
Fig. 10 Damage map at46 s and the crackbranching evolution around23 s ( = 0.0005 m)
the loading is, however, quasistatic, in contrast to ourdynamicallyinduced crack propagation. The trends ofthe peridynamic crack propagation speed results for allmodels are very similar to one another. This indicates convergence behavior for the crack speed, since thehorizon was reduced by half, and the computed crack-tip propagation speeds did not change by much. Asobserved in Fig. 11d, the fluctuations for the coarsestmodel (blue triangles in Fig. 11d) are larger than inother fine models (green squares and orange circles inFig. 11d). The main reason for the larger fluctuation isthat, for the coarsest model, the crack advances by onlya few nodes between the data dumps, while in the finermodels the resolution is improved and the number ofachievable speed levels is increased.
We next compare the ratios of the numerical and theexperimental maximum crack propagation speeds tothe Rayleigh wave speed. An approximate expressionfor the Rayleigh wave speed cR (Graff 1975) is
cRc2
= 0.87 + 1.121 + (13)
where is the Poisson ratio and the shear wave speed c2is given by c2 =
. We select the maximum com-
puted crack speed value at 24 s from the numericalresult with the smallest horizon model (see Fig. 11d).
In Table 2, the ratio of this numerical maximum prop-agation speed to the Rayleigh wave speed cR is com-pared with the ratio of the experimentally measuredmaximum fracture speed (Bowden et al. 1967) for thesoda-lime glass material.
The observation in Sect. 4.2 about how wave reflec-tions from the boundaries affect the crack propagationpath also explains why the branching angles seen inBowden et al. (1967) are different from the ones weobtained here (for the soda-lime glass). The geometryused here is different from the one used in Bowden et al.(1967), where the notch is a short one, running parallelto the short side of the plate, the side boundaries arefarther away than in our case where the notch is longand parallel to the long side of the plate. The differentgeometry will strongly influence the propagation speedin the dynamic loading case since the stress waves aresupplying energy in the fracture region and that hasbeen observed to influence both the shape of the crackpath and the crack propagation speed (Ravi-Chandarand Knauss 1984b).
The results obtained with the finest horizon (andgrid spacing) give a maximum crack propagation speedvalue that is about 6% larger than the experimen-tally measured maximum crack speed for soda-limeglass of 1580 m/s (see Bowden et al. 1967). These
123
240 Y. D. Ha, F. Bobaru
Fig. 11 Crack paths andcrack propagation speedsfor soda-lime glass (for-convergence with m = 4).a Crack path at 40 s( = 0.002 m); b Crack pathat 40 s ( = 0.001 m);c Crack path at 40 s( = 0.0005 m); d Crackpropagation speed for threedifferent horizons;e Close-up at 20.5 s for thefinest horizon; f Close-up at21.5 s for the finesthorizon
Table 2 The ratios ofnumerically computed andexperimental maximumfracture speeds to theRayleigh wave speed
Fracture speed, V (m/s) V/cR
Peridynamics 1679 0.53
Experiment (Bowden et al. 1967) 1580 0.50
encouraging results, however, have to be understoodin context of the different type of loading conditionsused in the computations compared with the setup inBowden et al. (1967). Further comments and analysison this subject are given in Ha et al. (2010). We alsonote that here we use a constant fracture energy model.This may not be the case in reality where the criticalfracture energy can change with, for example, the speedof crack propagation. In Dll (1975), for instance, the
fracture energy is measured to depend on the propaga-tion velocity. This issue of the dependence of the frac-ture energy on the crack propagation speed and/or thelocal damage is also discussed, from the point of viewof experiments, in the more recent review article (Ravi-Chandar 1998). In Ha and Bobaru (2010), we report onresults that also use a modified critical relative elon-gation for damaged nodes so that nodes with damagelevels over a certain value have a larger critical relative
123
Studies of dynamic crack propagation 241
elongation. This, in effect, implements a change inthe critical fracture energy depending on the damagelevel at a particular point in the material. The influenceof using a damage-dependent critical relative elonga-tion on the crack propagation speed is discussed inHa and Bobaru (2010). This modification has beenobserved (Silling 2005) to give better results in frag-mentation problems. Without the damage-dependentcritical elongation model, peridynamics would create alot of smaller fragments, while using this modification,the number and size distribution of fragments matchexperimental observations.
We also note that the crack speed profiles have avery similar pattern with the experimental speed pro-file shown in Fig. 11 in reference (Field 1971). We nowquote from page 19 in Field 1971 which describes theexperimental observations of crack branching: Thetransition region and branch occur when the crack hasreached a high proportion of its maximum velocity. Thefirst serious roughening of the fracture surface gave aslight, but detectable, slowing of the crack. Followingcrack bifurcation the surfaces of the two new cracksnormally appear mirror smooth, indicating a somewhatlower velocity than in the transition region. However,the branching does not cause the fracture front veloc-ity to drop to zero or even near it. This is demonstratedby the fracture of toughened glass where the velocityof the front progresses at a relatively uniform veloc-ity of nearly 1,500m/s The peridynamic results inFig. 11 match surprisingly well with each and everyobservation in the quoted text above. Small fluctua-tions of the speed profile, and a slowing of the crack,appear around 1416 s (see Fig. 11d), which is simi-lar to what happens during the initial roughening inFig. 11 in Field (1971). Please note that our model it toocoarse to capture actual roughening of the crack sur-faces. Indirect evidence of roughness, however, may beobserved from our computations, and this is discussednext. The more severe roughening discussed in Field(1971) is seen in Fig. 11e,f, as a wider damage zone.This happens just before branching of the crack, thesame as in the experiments. At that stage, the crackhas been moving at a high proportion of its maximumvelocity. After branching, we observe a small drop inthe propagation velocity, and the damage region alongthe crack paths is indicative of smooth crack surfacesof each branch (see Fig. 11f).
It is interesting to note the correlation between thestress waves that continue to propagate and reflect from
the boundaries and the crack propagation speed. Themore recent experimental evidence points towards thisinteraction as one main cause of crack branching (seeRavi-Chandar 1998; Ravi-Chandar and Knauss 1984b).Our peridynamic simulations confirm this point of view.It appears that the speeding, slowing down, speeding,and then slowing slightly in the region of branching, ofthe crack tip during the time interval from 5 to 20 s isdirectly caused by the way the elastic strain energy con-centrates towards (which results in speedingof thecracktip) or disperses away (which results in slowing down ofthecrack tip) fromthe frontof thecrackpath.This is eas-ier to see in a movie of the dynamic crack propagationprocess (Ha et al. 2010).
4 Numerical results for different micro-modulusfunctions and different materials at higherstress levels
4.1 Constant versus conical micro-modulusfunctions
In the following we compare the results for two differ-ent micro-modulus functions. The tests are performedusing the soda-lime glass material properties, and thenumerical model is the same except for the type ofmicro-modulus functions: the constant micro-modulus(Eq. 6) and the conical micro-modulus function (Eq. 7).
The peridynamic models have = 1 mm and gridspacing x = 0.25 mm (65,448 nodes). The Veloc-ityVerlet algorithm is used for the time integrationwith a uniform time step size of 25 ns. The uniformtensile stress = 10 MPa is applied for the model inFig. 1. In Fig. 12 we compare the crack branching pathsat 50 s for the constant and conical micro-modulusfunctions. We observe very similar branching pathsup to a point when, due to the different reflectionswaves produced, the branches in the conical micro-modulus case splay out more than in the constantmicro-modulus case. Thus, the particular shape of themicro-modulus function influences the crack propa-gation path, but to a small extent. In Xie (2005), itwas shown that a flux-corrected transport (FCT) algo-rithm can eliminate the ripples behind a shock wave ina peridynamics simulation. The FCT algorithm is notused in this paper and thus the ripples behind the shockwaves are not eliminated. Since a different micro-mod-ulus function creates different dispersion curves (see
123
242 Y. D. Ha, F. Bobaru
Fig. 12 Crack paths for different micro-modulus functions at 50 s ( = 0.001 m, x = 0.00025 m) for soda-lime glass. a Solutionwith conical micro-modulus; b Solution with constant micro-modulus
Fig. 13 Crack paths for two different materials under higher loading conditions ( = 0.001 m, x = 0.00025 m). a Damage map forsoda-lime glass at 28 s; b Damage map for Duran 50 glass at 32 s
Silling 2000), the oscillations behind the shock wave inour computations (see Fig. 4) interfere with the crackpath and create differences in the propagation direc-tions between the two models. Note, however, that thecrack propagation speeds for the two different cases arevery close to one another.
4.2 Crack branching patterns for two differentmaterials under higher stress levels
We compare the crack branching patterns between thesoda-lime glass and Duran 50 glass under higher load-ing conditions. The peridynamic models for both mate-rials have = 1 mm and grid spacing x = 0.25 mm(65,448 nodes). The VelocityVerlet algorithm with auniform time step size of 25 ns is employed, and theuniform tensile stress = 24 MPa is applied suddenlyat the initial time-step. In Fig. 13, we observe thatcascading branching takes place for the soda-limematerial, while for the Duran glass, under these partic-ular conditions, the branching events attempted afterthe main one are arrested. We also note the curving ofthe secondary branches for the soda-lime case. Exper-imental confirmation of this phenomenon is given inRavi-Chandar and Knauss (1984b), for example. Thereason for both the arrested branches and the crack pathcurving rests with the particular way the stress waves
are moving through each material and reflecting fromthe boundaries.
A close examination of the strain energy maps dur-ing the crack propagation process clearly shows howthe strain elastic energy concentrates in certain regionsand the particular incident angle at which the elasticenergy waves meet the crack tip can result in bendingthe crack path for the soda-lime case (see Fig. 14a)or in arresting the propagation of secondary branchesfor the Duran glass case (see Fig. 14b). In Fig. 14,the elastic strain energy is plotted on the top row fig-ures for areas around the front of the crack propagationpath at two different times (21 and 22 s for soda-limeglass and 24 and 26 s for Duran glass). The bottomrow of figures in Fig. 14, shows the damage index atsimilar time steps and at various degrees of close-upsaround the top-most branches. For the soda-lime glass(Fig. 14a), the reflection waves hit the crack tip of thesecond branching event at an inclined angle (see strainenergy at 21 s). This bends the top-most branch asseen from the sequence of plots at 23, 25, and 27 s, andin Fig. 13a at 28 s. For the Duran glass case (Fig. 14b),the reflection waves meet the crack tip at an angle thatsuppresses, or arrests, the top-most branch and its sym-metrical, lower-most branch.
We remark that in the soda-lime case, the con-ditions allow for yet another branching event fromsome of the secondary crack paths. Also, the thicker
123
Studies of dynamic crack propagation 243
Fig. 14 Elastic strainenergy around the crack tipareas (top row of figures)and damage maps (bottomrow of plots) at timescorresponding to thesecondary branching events.Left plots are for soda-limeglass, right plots are forDuran glass. a Soda-limeglass; b Duran 50 glass
damage zone following the primary branching eventfor the Duran glass indicates a rough zone where con-ditions where close to those that would produce branch-ing. The particular interaction of the crack path with thereflection stress waves arrested that branching eventbefore it happened. Later on, around 26 s, second-ary branching happens but some of the branches arearrested soon after forming, while the others continueto propagate (see Fig. 13b).
Note that here, as before, we used a constant fractureenergy that corresponds to that measured at branchingand reported in Dll (1975). A discussion about thesymmetry and the symmetry breaking in the peridy-namic simulations is included in Ha and Bobaru (2010).
5 Conclusions
In this paper we presented some detailed studies ofmodeling dynamic fracture and capturing crack branch-ing events in brittle materials using peridynamics. Theresults demonstrate that dynamic fracture phenomenaare captured by the peridynamic formulation very well.All the details of dynamic crack branching in brittlematerials reported in the experimental literature arerecovered by our peridynamic simulations, naturallyand without having to insert various special crack prop-agation criteria, for example, for when and how branch-ing should take place. In both the experiments and theperidynamic model, branching occurs in a region wherethe crack propagation speed reaches a high propor-tion of its maximum value. There is roughening beforebranching in the experiments and that is captured asa thicker damage zone ahead of the branching regionby the peridynamic simulations. There is a small, butdetectable, slowing of the crack propagation speed afterbranching in both the experiments and our computa-
tional results. There is cascade branching in the experi-ments when higher stress levels are attained before thecrack starts to propagate, and we also observed thatin our peridynamic solutions when we increased themagnitude of the applied loads.
Convergence in terms of the number of nodes cov-ered by the peridynamic horizon is obtained, and thecrack path and crack propagation speed stabilize, orconverge, once the horizon becomes of sub-millimetersize, for the sample that measured in centimeters. Asmall influence of the specific shape of the peridynam-ic micro-modulus function is observed on the crackpropagation path but not on the propagation speed.
Our results for this complex physical process shedlight over the question of why Molecular Dynamics(MD) simulations fail to correctly predict crack branch-ing: the phenomenon involves scales of the size of theentire structure since it is the propagation of the elasticstrain energy (stress waves) and their reflection from theboundaries of the structure that control the crack prop-agation process (in terms of the propagation speed andcrack path direction) in dynamic fracture. We also notethe correlation between the size of the horizon at whichthe peridynamic results appear to no longer change andthe characteristic interaction distance talked aboutin Streit and Finnie (1980), Ramulu and Kobayashi(1985). This issue requires further investigation whichwe plan for the future.
The overall trend of the crack propagation speedfrom our simulations showed a remarkable resem-blance to the experimental speed profiles reported byothers. We compared the maximum crack propaga-tion speed obtained with peridynamics with that fromthe experiments and the value, for the 0.5 mm horizoncase, was about 6% larger than the experimental valuefor soda-lime glass. While the loading conditions aredifferent (quasi-static in experiments, dynamic in our
123
244 Y. D. Ha, F. Bobaru
simulations), the result is remarkable given that theinput in our model was a constant value of the criticalfracture energy equal to that measured at crack branch-ing. In conclusion, peridynamics succeeds in correctlymodeling crack branching in brittle plates, one of themain open problems in modeling dynamic fracture.
Acknowledgments The authors would like to acknowledge thefinancial support from the Boeing Company (project manager:Dr. E. Askari) and from Sandia National Laboratories (projectmanager: Dr. S. A. Silling) without which this work would nothave been possible. Very useful discussions with Dr. M. L. Parksand Dr. S. A. Silling regarding time integration algorithms arealso gratefully acknowledged. The authors would also like tothank the two anonymous reviewers for their insightful com-ments. The computations in this paper have been completed usingfacilities at the University of Nebraska Holland ComputingCenter.
References
Belytschko T, Chen H, Xu J, Zi G (2003) Dynamic crack prop-agation based on loss of hyperbolicity and a new discontin-uous enrichment. Int J Numer Methods Eng 58:18731905
Bobaru F, Yang M, Alves LF, Silling SA, Askari E, Xu J(2009) Convergence, adaptive refinement, and scaling in 1Dperidynamics. Int J Numer Methods Eng 77:852877
Bolander JE Jr, Saito S (1998) Fracture analyses using springnetworks with random geometry. Eng Fract Mech 61:569591
Bowden FP, Brunton JH, Field JE, Heyes AD (1967) Controlledfracture of brittle solids and interruption of electrical cur-rent. Nature 216:3842
Buehler MJ, Abraham FF, Gao H (2003) Hyperelasticity gov-erns dynamic fracture at a critical length scale. Nature426:141146
Camacho GT, Ortiz M (1996) Computational modelling ofimpact damage in brittle materials. Int J Solids Struct33:28992938
Cox BN, Gao H, Gross D, Rittel D (2005) Review: moderntopics and challenges in dynamic fracture. J Mech PhysSolids 53:565596
Dll W (1975) Investigations of the crack branching energy. IntJ Fract 11:184186
Field JE (1971) Brittle fracture: its study and application. Con-temp Phys 12(1):131
Graff KF (1975) Wave motion in elastic solids. Dover, New YorkHa YD, Bobaru F (2009) Traction boundary conditions in
peridynamics: a convergence study. Technical reportDepartment of Engineering Mechanics, University ofNebraskaLincoln, Lincoln, Nebraska
Ha YD, Bobaru F (2010) The effect of damage-dependentfracture energy on symmetry-breaking in dynamic brit-tle fracture. Technical report, Department of Engineer-ing Mechanics, University of NebraskaLincoln, Lincoln,Nebraska.
Ha YD, Bobaru F, Parks ML (2010) Dynamic brittle fracture:crack branching predictions with peridynamics (submitted)
Hairer E, Lubich C, Wanner G (2003) Geometric numericalintegration illustrated by the Strmer/Verlet method. ActaNumer, 151
Livne A, Ben-David O, Fineberg J (2007) Oscillations in rapidfracture. Phys Rev Lett 98(12):124301
Ortiz M, Pandolfi A (1999) Finite-deformation irreversible cohe-sive elements for three-dimensional crack-propagationanalysis. Int J Numer Methods Eng 44:12671282
Rabczuk T, Belytschko T (2004) Cracking particles: a simplifiedmeshfree method for arbitrary evolving cracks. Int J NumerMethods Eng 61:23162343
Ramulu M, Kobayashi AS (1985) Mechanics of crack curvingand branchinga dynamic fracture analysis. Int J Fract27:187201
Ravi-Chandar K (1998) Dynamic fracture of nominally brittlematerials. Int J Fract 90:83102
Ravi-Chandar K, Knauss WG (1984a) An experimental inves-tigation into dynamic fracture: III. On steady-state crackpropagation and crack branching. Int J Fract 26:141154
Ravi-Chandar K, Knauss WG (1984b) An experimental investi-gation into dynamic fracture: IV. On the interaction of stresswaves with propagating cracks. Int J Fract 26:189200
Silling SA (2000) Reformulation of elasticity theory for discon-tinuities and long-range forces. J Mech Phys Solids 48:175209
Silling SA (2005) Fragmentation modeling with EMU. Tech-nical report, Computational Physics Department, SandiaNational Laboratories, Albuquerque, New Mexico
Silling SA, Askari E (2005) A meshfree method based on theperidynamic model of solid mechanics. Comput Struct83:15262535
Silling SA, Demmie P, Warren TL (2007a) Peridynamic sim-ulation of high-rate material failure, 2007 ASME appliedmechanics and materials conference, Austin, TX, June 6
Silling SA, Epton M, Weckner O, Xu J, Askari E (2007b) Peridy-namic states and constitutive modeling. J Elast 88:151184
Silling SA, Lehoucq RB (2008) Convergence of peridynamicsto classical elasticity theory. J Elast 93:1337
Silling SA, Weckner O, Askari E, Bobaru F (2009) Crack nucle-ation in a peridynamic solid. Int J Fract (this issue)
Song J, Areias PMA, Belytschko T (2006) A method fordynamic crack and shear band propagation with phantomnodes. Int J Numer Methods Eng 67:868893
Song JH, Wang H, Belytschko T (2008) A comparative study onfinite element methods for dynamic fracture. Comput Mech42:239250
Streit R, Finnie I (1980) An experimental investigation of crack-path directional stability. Exp Mech 20:1723
Xie W (2005) Peridynamic flux-corrected transport algorithm forshock wave studies. Master thesis, Department of Engineer-ing Mechanics, University of NebraskaLincoln, Lincoln,Nebraska
Xu XP, Needleman A (1994) Numerical simulations of fastcrack growth in brittle solids. J Mech Phys Solids 42:13971434
Zhou F, Molinari JF (2004) Dynamic crack propagation withcohesive elements: a methodology to address mesh depen-dency. Int J Numer Methods Eng 59:124
Zhou SJ, Lomdahl PS, Thomson R, Holian BL (1996) Dynamiccrack processes via molecular dynamics. Phys Rev Lett76(13):23182321
123
Studies of dynamic crack propagation and crack branching with peridynamicsAbstract1 Introduction1.1 Literature review of dynamic crack propagation1.2 Problem setup
2 The peridynamic formulation3 Numerical studies of convergence in dynamic crack branching3.1 The m-convergence study3.2 Crack path under changing horizon 3.3 Comparison of peridynamic crack propagation speed with experimental values
4 Numerical results for different micro-modulus functions and different materials at higherstress levels4.1 Constant versus conical micro-modulusfunctions4.2 Crack branching patterns for two different materials under higher stress levels
5 ConclusionsAcknowledgmentsReferences
/ColorImageDict > /JPEG2000ColorACSImageDict > /JPEG2000ColorImageDict > /AntiAliasGrayImages false /CropGrayImages true /GrayImageMinResolution 149 /GrayImageMinResolutionPolicy /Warning /DownsampleGrayImages true /GrayImageDownsampleType /Bicubic /GrayImageResolution 150 /GrayImageDepth -1 /GrayImageMinDownsampleDepth 2 /GrayImageDownsampleThreshold 1.50000 /EncodeGrayImages true /GrayImageFilter /DCTEncode /AutoFilterGrayImages true /GrayImageAutoFilterStrategy /JPEG /GrayACSImageDict > /GrayImageDict > /JPEG2000GrayACSImageDict > /JPEG2000GrayImageDict > /AntiAliasMonoImages false /CropMonoImages true /MonoImageMinResolution 599 /MonoImageMinResolutionPolicy /Warning /DownsampleMonoImages true /MonoImageDownsampleType /Bicubic /MonoImageResolution 600 /MonoImageDepth -1 /MonoImageDownsampleThreshold 1.50000 /EncodeMonoImages true /MonoImageFilter /CCITTFaxEncode /MonoImageDict > /AllowPSXObjects false /CheckCompliance [ /None ] /PDFX1aCheck false /PDFX3Check false /PDFXCompliantPDFOnly false /PDFXNoTrimBoxError true /PDFXTrimBoxToMediaBoxOffset [ 0.00000 0.00000 0.00000 0.00000 ] /PDFXSetBleedBoxToMediaBox true /PDFXBleedBoxToTrimBoxOffset [ 0.00000 0.00000 0.00000 0.00000 ] /PDFXOutputIntentProfile (None) /PDFXOutputConditionIdentifier () /PDFXOutputCondition () /PDFXRegistryName () /PDFXTrapped /False
/CreateJDFFile false /Description > /Namespace [ (Adobe) (Common) (1.0) ] /OtherNamespaces [ > /FormElements false /GenerateStructure false /IncludeBookmarks false /IncludeHyperlinks false /IncludeInteractive false /IncludeLayers false /IncludeProfiles false /MultimediaHandling /UseObjectSettings /Namespace [ (Adobe) (CreativeSuite) (2.0) ] /PDFXOutputIntentProfileSelector /DocumentCMYK /PreserveEditing true /UntaggedCMYKHandling /LeaveUntagged /UntaggedRGBHandling /UseDocumentProfile /UseDocumentBleed false >> ]>> setdistillerparams> setpagedevice